Dent Clin N Am 51 (2007) 433–451 Adhesion to Porcelain and Metal Raymond L. Bertolotti, DDS, PhD* University of California, San Francisco School of Dentistry, Parnassus Avenue, San Francisco, CA 94143, USA Advances in adhesion monomers and surface preparation techniques per-mit strong bonding of resins to metals and to porcelains. Most ‘‘pressed ce-ramics’’ bond in a manner similar to that of porcelains. The bond strengthsto these materials can easily exceed the typical bond of resin to phosphoric-acid–etched enamel . Using the strong bonds to these restorative mate-rials, many innovations in tooth-conservative procedures are possible. When we consider that tooth reduction correlates with need for subse-quent endodontic treatment , the preferred treatment option often isone that relies on minimal tooth reduction. Adhesion, with less need fortooth reduction, is a highly desirable shift away from tooth preparationfor mechanical retention. This paper ﬁrst presents some clinical examples where the use of adhe-sives clearly provides compelling advantages compared with mechanical re-tention and cementation. Then methods and materials to achieve resinadhesion to metal and porcelain are reviewed. Based on these methodsand materials and the author’s own clinical experience, speciﬁc adhesionprotocols are given for some complex clinical applications.The clinical advantages of using porcelain and metal adhesion If we examine the cross section of a typical molar (Fig. 1), the distancefrom the occlusal surface to the pulp chamber is about 7 mm. A 3-mm oc-clusal reduction therefore leaves about 4 mm of remaining dentin thickness(Fig. 2). On the other hand, axial reduction of 2 mm leaves !1 mm of re-maining dentin (Fig. 3). The 2-mm axial reduction is within current pressedceramic manufacturers’ instructions for tooth preparation. Raymond L. Bertolotti owns stock in Danville Materials Inc. * 188 Beechwood Drive, Oakland, CA 94618. E-mail address: firstname.lastname@example.org/07/$ - see front matter Ó 2007 Published by Elsevier Inc.doi:10.1016/j.cden.2006.12.003 dental.theclinics.com
434 BERTOLOTTI Fig. 1. Cross section of a molar. With porcelain, metal, and even dentin adhesion equivalent to etchedenamel adhesion, the obvious clinical application is the adhesion onlay.The onlay may be made of metal, porcelain, or pressed ceramic (Figs. 4and 5). In these examples shown in Figs. 4 and 5, there is no intentionallycut retention form (Fig. 6). The ‘‘preparation’’ of the teeth was actuallydone by the patient through years of abrasion. No additional tooth modiﬁ-cation was made before taking the ﬁnal impression. Last photographed at5 years and 3 months, this case remains successful after nearly 10 years. While metal adhesion onlays have been successful for many years , cli-nicians have been reluctant to place occlusal porcelain onlays on molars.Presumably the reluctance results from reports of clinical failure of all por-celain molar crowns. However, a recent study , where 2 mm of pressedceramic (Empress; Ivoclar/Vivadent, Schaan, Leichtenstein) was bondedto the occlusal surfaces of molars (partial onlays, not crowns), reported100% success at 33 months. These onlays used 2 mm of pressed ceramic,like those demonstrated on the previous case. The high success rate is Fig. 2. Shaded area shows 3-mm occlusal reduction.
PORCELAIN AND METAL 435 Fig. 3. Shaded area shows 3-mm occlusal reduction and 2-mm axial reduction.presumed to be due to the ceramic being placed in compression during func-tion, well supported by bonding to enamel and dentin. Another tooth-conserving example is the cantilevered adhesion bridge(Figs. 7–9) of porcelain fused to metal, bonded to enamel. This is similarto the ‘‘Maryland bridge’’ but the ‘‘Yamashita adhesion bridge’’ uses resis-tance channels placed in enamel . Such mesial and distal channels producea highly successful result  when the metal is bonded to phosphoric-acid–etched enamel. Porcelain veneers are a third compelling application of adhesives. The ad-herends are porcelain and enamel, porcelain and dentin, or porcelain andboth enamel and dentin. Veneers can be done successfully with minimal in-tra-enamel tooth reduction . The survival rate in most reports exceeds90% at 10 years. The high success rates can be attributed to durable bondingand support for the porcelain provided by tooth structures (Figs. 10–13). All the clinical examples illustrated above can generally be accomplishedin a straightforward manner by following manufacturers’ instructions for Fig. 4. Occlusal ‘‘adhesion onlays’’ of gold alloy and pressed ceramic.
436 BERTOLOTTI Fig. 5. Onlay 5 years and 3 months after completion. Fig. 6. Occlusal surface of cast with margins marked in red. Fig. 7. Completed Yamashita adhesion bridge bonded to enamel.
PORCELAIN AND METAL 437 Fig. 8. Retainer preparation using intra-enamel channels.the adhesive. While sometimes not as straightforward, porcelain repairs canalso be highly successful. Some repairs require bonds to several dissimilarsurfaces. After the discussion of metal adhesion and porcelain adhesion,some repair applications are illustrated and speciﬁc clinical protocols givenfor adhesion to multiple surfaces.Metal adhesionMechanical retention Adhesion to metal has long been a goal in dentistry. Resin-bonded‘‘Rochette’’  retainers were described in 1973. Retention was provided me-chanically by composite resin locking into tapered perforations in the metal.A diﬀerent approach to mechanical retention, using electrolytic etching toproduce a microscopically retentive surface on the entire inner surface ofthe metal, was subsequently reported . This etched metal is used forwhat is usually called the ‘‘Maryland bridge.’’ Using the microscopic ap-proach, two critical factors for successful adhesion to a metal substrate Fig. 9. Adhesion retainer on cast, lingual view.
438 BERTOLOTTIFig. 10. Intra-enamel tooth preparations for a conventional veneer on the lateral incisor and‘‘sectional’’ mesial veneer on the cuspid.are (1) using an adhesive liquid with excellent wetting characteristics and (2)providing a high-energy metal surface to promote good wetting.Substrate modiﬁcation Several researchers took a diﬀerent approach to modifying the adherendmetal surface. By itself or in conjunction with other procedures, sandblast-ing with aluminum oxide has become an almost universal procedure. Sand-blasting with aluminum oxide can be done extraorally or intraorally.Sandblasting provides a fresh and uncontaminated surface that is high insurface energy and can be easily wetted by suitable metal bonding agents.Some other reported adherend modiﬁcations are high-temperature oxida-tion, immersion in an oxidizing agent, anodizing, and alloying the surfacewith a liquid gallium–tin alloy. In contemporary dental practices, thesemodiﬁcations do not appear to be used often. A diﬀerent and more popularapproach is adding a SiOx-C coating by injecting a solution through a specialﬂame . Then a special silane is applied to the coated surface. This Fig. 11. Cast showing tooth preparations by marked margins.
PORCELAIN AND METAL 439 Fig. 12. Immediate result after veneers were bonded.method is known as Silicoater (Heraeus Kulzer, Hanau, Germany). A morerecent approach, widely used, is known commercially as Rocatec in the lab-oratory and CoJet chairside (3M ESPE AG, Seefeld, Germany). With thismethod, a tribochemical silica coating is sandblasted onto the metal surfaceto provide ultraﬁne mechanical retention. When treated with the silica-coat-ing system, the surface is not only ‘‘abraded,’’ but becomes embedded witha silica coating derived from silica-coated aluminum oxide particles. Metaland many other surfaces may be abraded with 30-mm grain size CoJet-Sand. Intraoral application is done with an intraoral sandblaster (Fig. 14),such as the Microetcher (Danville Materials, San Ramon, California). Aspecialized silane coupling agent is then applied.Chemical modiﬁcation of ﬁlled resins Modiﬁcation of the chemistry of resin to create aﬃnity for metals is an-other approach taken to strongly adhere resins to metals. Following the de-velopment in 1978 of a new adhesive monomer, 4-META , a commercial Fig. 13. Veneer 8.5 years after bonding.
440 BERTOLOTTI Fig. 14. Microetcher ERC II sandblaster with intraoral, contra-angle tip attached.powder and liquid acryliclike product, Super Bond C&B (Sun Medical Co.,Ltd., Kyoto City, Japan) was introduced in 1982 for adhesion to dental al-loys and to tooth structures . To improve mechanical properties of theadhesive resin and to change the handling characteristics, another approachwas taken, which resulted in the product Panavia Ex (Kuraray, Osaka, Ja-pan) . It is a low-viscosity, quartz-ﬁlled composite resin containinga phosphate monomer known as M-10-P. Panavia is known to bond wellto sandblasted base metals, but its bond to noble metals decreases whenstored in water. To overcome this bond instability, the manufacturer devel-oped a laboratory tin–plating apparatus, known as the Kura-Ace. It is usedon noble metal alloys after sandblasting. Subsequently, two manufacturersproduced portable tin platers capable of intraoral use . These are Kura-Ace Mini (Kuraray) and Microtin (Danville Materials). A more recent prod-uct, similar to Panavia but using a diﬀerent adhesion monomer, is Bistite IIDC (Tokuyama, Tokyo, Japan). Tin plating has been challenged by the useof metal primers, presumably because metal primers are more expedient toFig. 15. Hydroxyethyl methacrylate on freshly sandblasted gold alloy surface. (Courtesy ofTom Blake, San Ramon, CA.)
PORCELAIN AND METAL 441Fig. 16. Hydroxyethyl methacrylate on 24-hours–aged sandblasted gold alloy surface. (Courtesyof Tom Blake, San Ramon, CA.)use. One recent study  compared the adhesive primers Alloy Primer(Kuraray), Metal Primer II (GC America, Alsip, Illinois), and Metaltite(Tokuyama) and the resin cements Bistite II (Tokuyama), Panavia F andSuper-Bond C&B. All combinations appear to be potentially successfulfor the bonding of prosthodontic restorations, although there were reporteddiﬀerences in bond stability.Unﬁlled ‘‘universal’’ bonding resins As opposed to using a chemically modiﬁed ﬁlled resin, another method isto use a ‘‘universal’’ bonding agent, such as the All-Bond 2 System (Bisco,Inc., Schaumburg, Illinois), and then add a layer of ﬁlled resin. Primer B ofthe All Bond 2 System can function as a metal primer . According to themanufacturer, when using the All-Bond 2 System, tin plating does not im-prove the bond strength of composite resin to sandblasted noble alloys. Sim-ilarly Clearﬁl (Kuraray) adhesives, such as Photo Bond and SE Bond,provide excellent metal bonding agents owing to the inclusion of the sameadhesion monomer (M-10-P) as in Panavia. Fig. 17. Tin plate on sandpaper-treated gold alloy.
442 BERTOLOTTI Fig. 18. Tin plate on gold alloy sandblasted with aluminum oxide.Metal surface preparation Contaminants on metal surfaces reduce surface energy and may compro-mise the bond strength to all resins. Sandblasting can remove such contami-nants, creating a fresh, clean, and microscopically irregular surface with highsurface energy. A high-energy surface is more wettable than a low-energysurface. An investigator, Tom Blake, looked at the eﬀect of a delay after sand-blasting, before the adhesive was applied. Blake, Director of Research atDanville Engineering, reported to the author in 2006 that the delay has a sig-niﬁcant eﬀect on wetting. Figs. 15 and 16 show the wetting of hydroxyethylmethacrylate (HEMA), a component of many bonding agents, at two elapsedtimes after sandblasting. When a measured drop of HEMA was applied to the‘‘freshly’’ sandblasted gold alloy surface, a low contact angle and goodwetting was observed. When the time was delayed for 24 hours aftersandblasting, the HEMA did not wet as well, presumably because anabsorbed layer on the metal surface lowered the surface energy. Fig. 19. Hydroﬂuoric-acid–etched porcelain. (Courtesy of Tom Blake, San Ramon, CA.)
PORCELAIN AND METAL 443 Fig. 20. Three components of Clearﬁl Porcelain Bond, which are mixed before use. Clearly there is an advantage to having sandblast capability at chairsideto freshly sandblast metals just before applying adhesive. It is common fordentists in North America to use such sandblasting. Outside North America,use is far lower but, according to the manufacturer of CoJet, many dentistsworldwide use similar sandblasters to apply CoJet sand. Sandblasting is generally used before tin plating of noble metals. In addi-tion to providing added mechanical retention, the sandblasting activates themetal surface and makes it more receptive to tin plating. Somewhat analo-gous to the above HEMA wetting experiment is the tin plating activity onthe sandblasted surface compared with a surface polished with ﬁne abrasivepaper. Plating tin onto an aluminum-oxide–sandblasted gold alloy surfaceresults in tiny crystals covering the entire surface. In contrast, tin plating af-ter abrasive paper treatment results in large crystals growing out of a fewactive spots. Therefore, it appears that the best tin plating results by electro-plating a freshly sandblasted surface (Figs. 17 and 18). Fig. 21. Before repair.
444 BERTOLOTTI Fig. 22. Isolation. The character of the tin crystal may play a role in the adhesion of resinsto tin-plated metals. It may be that tin provides the enhanced mechanicalretention or that a chemical bonding link to resin is established. In anyevent, the author’s clinical experience with Panavia on tin-plated goldstrongly suggests that the tin-plated metal-to-Panavia bond is superior tothe Panavia-to-enamel bond. Debonds, although rare, invariably occur ad-hesively at the enamel-to-resin interface when Panavia is properly used. Thisobservation is supported by shear bond testing . It is interesting to notethat ‘‘onlays’’ bonded with Panavia, when stressed to failure in a dislodge-ment test, broke the teeth cohesively rather than debond . In summary, metal adhesion relies on an adhesive liquid with excellentwetting characteristics and a high-energy metal surface to promote goodwetting. Modiﬁcation of the adherend metal and modiﬁcation of resinchemistry both play roles in achieving high bond strength and durability,important for clinical success. Fig. 23. Sandblasting of porcelain and metal with aluminum oxide.
PORCELAIN AND METAL 445 Fig. 24. Phosphoric acid cleansing of repair surface, followed by wash and dry.Porcelain adhesionEtchable porcelains and pressed ceramics ‘‘Feldspathic’’ porcelain (eg, Ceramco 2; Dentsply, York, Pennsylvania)and pressed leucite– or lithium-disilicate–reinforced ceramics (eg, IPS Em-press and Empress II; Ivoclar/Vivadent) are treated in similar ways beforebonding. Being etchable with hydroﬂuoric acid and other ﬂuorides (eg, acid-ulated phosphate ﬂuoride and ammonium biﬂuoride), a strong resin bondcan result from mechanical interlocking. Hydroﬂuoric acid (HF) solutionsbetween 2.5% and 10% applied for 2 to 3 minutes are commonly used onporcelain and many pressed ceramics. The exact etching time depends onthe substrate and the acid concentration. The glassy matrix of the porcelainis selectively removed and crystalline structures are exposed, creating a roughsurface (Fig. 19). Some low-fusing porcelains and pressable ceramics do notetch well due to the low volume of acid-resistant crystalline structure. Generally, etching is followed by application of a silane coupling agent.In addition to enhancing the wettability of the surface, the silane providesa chemical bond to the silica-based ceramic surface. Being bifunctional Fig. 25. Application of three-component Clearﬁl Porcelain Bond.
446 BERTOLOTTI Fig. 26. Opaquer being applied, followed by light activation.molecules, silanes bond to the silicon dioxide as well as copolymerize withthe resins in the composite bonding agent that is subsequently applied.However clinical success has been reported  for bonding of etched por-celain veneers that had no silane applied. Presumably that success can be at-tributed to suﬃcient mechanical interlocking to resin created by etching ofthe porcelain surface.Nonetchable ceramics Nonetchable aluminum oxide or zirconium oxide surfaces (eg, Inceram;Vident, Brea, California) are not to be confused with HF-etchable porce-lains. Since these oxides are not etchable with HF, they will not achievea strong and stable bond by the same method as that used for porcelain. Instead, certain adhesion monomers, such as M-10-P in Panavia,may be used to create a strong and stable bond. Likewise, Rocatec and Co-Jet are known to promote adhesion to these surfaces . A little-known  product line called Clearﬁl (Kuraray) bonds silica-based ceramics without the need for HF etching; it only uses sandblasting. Fig. 27. Application of composite, followed by light activation and polishing.
PORCELAIN AND METAL 447 Fig. 28. Completed repair.The porcelain bonds are equal to those achieved by HF etching followed bythe best silanes . Clearﬁl products are not the only ones capable of suchporcelain bonds. However, unlike the other products, Clearﬁl products alsosimultaneously (with only one mix of material) bond to metals, etchedenamel, and etched dentin. Clinical use of one of these products, ClearﬁlPhoto Bond base and catalyst mixed with Clearﬁl Porcelain Bond Activator(Fig. 20), is illustrated later for simultaneous bonding to multiple substrates.This combination of three components is known as Clearﬁl Porcelain Bond.All Clearﬁl products are also capable of bonding to alumina and zirconiadue to the Panavia monomer M-10-P in their formulas.Complex clinical applicationsPorcelain repair Clinicians often face challenging cases where adhesion to multiple sur-faces is required. Such a case is illustrated by the fractured porcelain on Fig. 29. Tooth loss, before replacement.
448 BERTOLOTTI Fig. 30. Porcelain removed from distal abutment.a ﬁve-unit ﬁxed partial denture (Fig. 21). Successful repair with compositeresin requires simultaneous adhesion to a base metal alloy and also to por-celain. Many similar situations also involve adjacent dentin and enamel (eg,an endodontic opening in a crown) where there would be metal, porcelain,dentin, and, perhaps, enamel. Illustrated below is a clinical example where Clearﬁl Photo Bond (a sort of dual-cure ‘‘prime and bond’’) mixedwith the Clearﬁl Porcelain Bond Activator is used to bond to all surfacessimultaneously (Figs. 22–28).Pontic addition Another challenging situation is the loss of a tooth adjacent to a relativelynew three-unit ﬁxed partial denture. With the capability for intraoral sand-blasting and tin plating, the replacement of this lost tooth is easy. Porcelainis removed from the distal tooth of the existing restoration to create a prep-aration that will draw occlusally, in alignment with the preparation of thenatural tooth distal abutment. A three-unit repair is prepared in the Fig. 31. Repair base metal casting with porcelain applied.
PORCELAIN AND METAL 449 Fig. 32. Microtin plater with contact ring for intraoral connection.laboratory. Since the existing metal is a noble alloy, sandblasting and intrao-ral tin plating is used to condition the prepared abutment. The repair castingonly requires sandblasting since it is fabricated with a base metal alloy. Thenatural tooth abutment distal to the missing tooth is treated with self-etch-ing ED Primer (Kuraray) before bonding with Panavia F. The Panavia Fbonds to the ED Primer as well as to both conditioned metals (Figs. 29–34).Other uses Following techniques similar to those used in the aforementioned toothreplacement, a procedure for replacement of a missing acrylic facing ona gold-acrylic crown has been published . Again, intraoral sandblastingand tin plating were used to condition the metal. Panavia was then used tobond a fully opaqued Artglass (Heraeus Kulzer) facing the conditionedmetal. Using similar technology, modiﬁcation of existing gold occlusals byintraoral bonding of new occlusal gold was reported . Fig. 33. Intraoral tin plating of sandblasted metal surface.
450 BERTOLOTTI Fig. 34. Tooth replacement complete.Summary Development of adhesives and modiﬁcation of adherends have madeit possible to bond to metal and porcelain with enamel-like adhesion. Max-imum tooth conservation is the compelling advantage in using these mate-rials and methods.References  Bertolotti RL, Lacy AM, Watanabe LG. Adhesive monomers for porcelain repair. Int J Prosthodont 1989;2:483–9.  Zollner A, Gaengler P. Pulp reactions to diﬀerent preparation techniques on teeth exhibiting periodontal disease. J Oral Rehabil 2000;27:93–102.  Uchiyama Y. Adhesion in prosthetic restorations. In: Gettleman L, Vrijhoef MMA, Uchiyama Y, editors. Adhesive prosthodontics. Chicago (IL): Academy of Dental Mate- rials; 1986. p. 21–31.  Guess PC, Stappert CF, Strub JR. Clinical study of press ceramic and cerec partial coverage restorations. Presented at the International Association for Dental Research 84th General Session. Brisbane, Australia, June 28–July 1, 2006. Abstract number 1639.  Yamashita A, Yamani T. Adhesion bridge, background and clinical procedure. In: Gettle- man L, Vrijhoef MMA, Uchiyama Y, editors. Adhesive prosthodontics. Chicago (IL): Acad- emy of Dental Materials; 1986. p. 61–76.  Botelho MG, Lai SCN, Ha WK, et al. Two-unit cantilevered resin-bonded ﬁxed partial den- turesda retrospective, preliminary clinical investigation. Int J Prosthodont 2000;13:25–8.  Freedman MJ. Porcelain veneer restorations: a clinician’s opinion about a disturbing trend. J Esthet Restor Dent 2001;13:318–27.  Rochette AL. Attachment of a splint to enamel of lower anterior teeth. J Prosthet Dent 1973; 37:28–31.  Livaditis GL, Thompson VP. Etched castings: an improved retentive mechanism for resin- bonded retainers. J Prosthet Dent 1982;47:52–8. Vojvodic D, Predanic-Gasparac H, Brkic H, et al. The bond strength of polymers and metal surfaces using the ‘silicoater’ technique. J Oral Rehabil 1995;22:493–9. Takeyama M, Kashibuchi S, Nakabayashi N, et al. Studies on dental self-curing resins. Adhesion of PMMA with bovine enamel or dental alloys. Shika Rikogaku Zasshi 1978; 19(47):179–85 [in Japanese].
PORCELAIN AND METAL 451 Nakabayashi N, Takeyama M, Kojima K, et al. Studies on dental self-curing resinsdadhe- sion of 4-META/MMA-TBB resin to pretreated dentine. Shika Rikogaku Zasshi 1982; 23(61):29–33 [in Japanese]. Wada T. Development of a new adhesive material and its properties. In: Gettleman L, Vrijhoef MMA, Uchiyama Y, editors. Adhesive prosthodontics. Chicago (IL): Academy of Dental Materials; 1986. p. 9–19. Yoshida K, Kamada K, Sawase T, et al. Eﬀect of three adhesive primers for a noble metal on the shear bond strengths of three resin cements. J Oral Rehabil 2001;28:14–9. Cinione FA, Stojkovich L, Suh BI. Resin:metal adhesion and the all bond 2 system. Esthetic Dent Update 1993;4:38–47. Freedman MJ. A 15-year review of porcelain veneer failure: a clinicians observations. Com- pendium Cont Dental Educ Dent 1998;19:625–8, 630, 632. Kern M, Thompson VP. Bonding of glass inﬁltrated alumina ceramic: adhesive methods and their durability. J Prosthet Dent 1995;73:240–9. Bertolotti RL. Bonding to porcelain (forum). Practical Periodontics and Aesthetic Dentistry 2005;17:232. Llobell A, Nichols JI, Kois JC, et al. Fatigue span of porcelain repair systems. Int J Prostho- dont 1992;5:205–13. Bertolotti RL, Miller D. Gold-acrylic facing replaced by intraoral bonding of a polyglass: a case report. Quintessence Int 1999;30:557–9. Bertolotti RL, DeLuca SS, DeLuca S. Intraoral metal adhesion utilized for occlusal rehabil- itation. Quintessence Int 1994;25:525–9.